Table 82. Continued. 









Depth 

 (ft) 



Corrosion 



■ 



Alloy 



Environment" 



Exposure 



(day) 



Rate 

 (mpy) 



Type 



Source 6 



5Al-2.5Sn rf 



W 



398 



5 



0.0 



NC 



CEL (4) 



5A1-2.5SI1* 



W 



398 



5 



0.0 



NC 



CEL(4) 



5Al-2.5Sn J 



w 



540 



5 



0.0 



NC 



CEL (4) 



5Al-2.5Sn ? 



w 



540 



5 



0.0 



NC 



CEL (4) 



5Al-2.5Sn tV 



w 



588 



5 



0.0 



NC 



CEL (4) 



7Al-2Cb-lTa rf 



w 



189 



5,900 



0.0 



NC 



CEL (4) 



7Al-2Cb-lTa e 



w 



189 



5,900 



0.0 



NC 



CEL (4) 



7Al-2Cb-lTa rf 



s 



189 



5,900 



0.0 



NC; BD 



CEL (4) 



7Al-2Cb-lTa' ? 



s 



189 



5,900 



0.0 



NC; BD 



CEL (4) 



7Al-2Cb-lTa' y 



w 



181 



5 



0.0 



NC; FS 



CEL (4) 



7Al-2Cb-lTa 6 ' 



w 



181 



5 



0.0 



NC;FS 



CEL (4) 



7Al-2Cb-lTa rf 



w 



398 



5 



0.0 



NC 



CEL (4) 



7Al-2Cb-lTa e 



w 



398 



5 



0.0 



NC 



CEL (4) 



7Al-2Cb-lTa d 



w 



540 



5 



0.0 



NC 



CEL (4) 



7Al-2Cb-lTa i? 



w 



540 



5 



0.0 



NC 



CEL (4) 



7Al-2Cb-lTa rf 



w 



588 



5 



0.0 



NC 



CEL (4) 



7Al-2Cb-lTa e 



w 



588 



5 



0.0 



NC 



CEL (4) 



4A1-3MO-1V 



w 



123 



5,640 



0.0 



NC 



NADC (7) 



4AI-3Mo-lV 



w 



403 



6,780 



0.0 



NC 



NADC (7) 



4A1-3M0-1V 



s 



403 



6,780 



0.0 



NC; BD 



NADC (7) 



4Al-3Mo-lV 



w 



751 



5,640 



0.0 



NC 



NADC (7) 



4Al-3Mo-lV 



s 



751 



5,640 



0.0 



NC; BD 



NADC (7) 



4Al-3Mo-lV 



w 



1,064 



5,300 



0.0 



NC 



CEL (4) 



4 Al- 3 Mo- IV 



w 



1,064 



5,300 



0.0 



NC 



NADC (7) 



4Al-3Mo-lV 



s 



1,064 



5,300 



0.0 



NC; BD 



NADC (7) 



4A1-3MO-1V 



w 



197 



2,340 



0.0 



NC 



NADC (7) 



4A1-3MO-1V 



s 



197 



2,340 



0.0 



NC; BD 



NADC (7) 



4A1-3MO-1V 



w 



402 



2,370 



0.0 



NC 



CEL (4) 



4A1-3MO-1V 



s 



402 



2,370 



0.0 



NC 



CEL (4) 



8'Mn 



w 



402 



2,370 



0.0 



NC 



CEL (4) 



8 Mn 



s 



402 



2,370 



0.0 



NC 



CEL (4) 



140 A 



w 



1,064 



5,300 



0.0 



NC 



CEL (4) 



7Al-12Zr 



w 



123 



5,300 



<0.1 



NC 



NADC (7) 



6A1-4V 



w 



123 



5,640 



<0.1 



NC 



NADC (7) 



6A1-4V 



w 



123 



5,640 



0.18 



NC 



MEL (5) 



6A1-4V 



w 



123 



5,640 



0.0 



NC 



CEL (4) 



6AI-4V* 



w 



123 



5,640 



0.0 



NC 



CEL (4) 



Continued 



230 



